Organic and Plastic Solar Cells Jenny Nelson, Centre for Electronic Materials and Devices, Department of Physics, Imperial College London, UK
1 2 3
Introduction Organic Photovoltaic Materials Principles of Operation and Device Concepts 3.1 Homojunctions 3.2 Heterojunctions 3.3 Dispersed Heterojunctions 4 Leading Device Designs 5 Challenges in Materials and Device Design 5.1 Light Harvesting 5.2 Improving Charge Transport 5.3 Control of Morphology 5.4 Understanding Function 6 Organic Photovoltaic Modules 7 Production Issues 7.1 General Issues 7.2 Production Processes for Molecular Films 7.3 Batch Production Processes for Polymer Films 7.4 Continuous Production Processes for Polymer Films 8 Performance and Stability 9 Conclusions Acknowledgements References
420 420 421 421 423 423 424 426 428 429 430 432 434 435 435 436 437 438 440 441 442 442
Solar Ceils: Materials, Manufacture and Operation
1 Introduction The last three years have seen an unprecedented growth of interest in solar cells made from organic electronic materials. This is due partly to the rapid growth of the photovoltaic market, which has stimulated research into longer term, more innovative photovoltaic technologies, and partly to the development of organic electronic materials for display applications. Rapid progress in optoelectronic molecular materials has introduced a range of potential new photovoltaic materials, as well as an improved understanding of the capabilities of such materials and confidence in their application. For a review see [ 1 ]. Organic materials are attractive for photovoltaics primarily through the prospect of high throughput manufacture using processes such as reel-to-reel deposition. Additional attractive features are the possibilities for ultra thin, flexible devices which may be integrated into appliances or building materials, and tuning of colour through chemical structure. The field has made impressive progress since the late 1990s. At the time of writing, solar power conversion efficiencies of over 3% have been reported for four distinct classes of organic solar cell, a growing range of new photovoltaic materials have been studied and increasing numbers of research groups and companies have declared an interest in'soft' solar cells [2-4]. Unlike other photovoltaic technologies featured in this handbook, organic or 'plastic' solar cells are far from commercialisation. It is not known which, if any, of several different materials systems and cell designs will prevail and there is no experience in module production. In this chapter, we will discuss the principles of organic electronic materials and the ways in which they differ from inorganic photovoltaic materials, the range of device concepts, the most efficient device designs and the main challenges in increasing efficiency. Possible production and processing technologies are discussed, but the practical details are largely speculative.
2 Organic Photovoltaic Materials Organic electronic materials are conjugated solids where both optical absorption and charge transport are dominated by partly delocalised n and rr* orbitals. Candidates for photovoltaic applications include crystalline or polycrystalline films of 'small molecules' (conjugated molecules of molecular weight of a few 100), amorphous films of small molecules prepared by vacuum deposition or solution processing, films of conjugated polymers or oligomers processed from solution, and combinations of any of these either with other organic solids or with inorganic materials. A comprehensive discussion of the development of organic solids for photovoltaic applications is given by Halls . Organic photovoltaic materials differ from inorganic semiconductors in the following important respects. Photogenerated excitations ('excitons') are strongly bound and do not spontaneously dissociate into charge pairs. (Dissociation requires an input
IIe-2- Organic and Plastic Solar Cells 421
9 9 9 9 9
of energy of ~ 1 0 0 meV compared to a few meV for a crystalline semiconductor.) This means that charge carrier separation generation does not necessarily result from the absorption of light. Charge transport proceeds by hopping between localised states, rather than transport within a band, which results in low mobilities. The spectral range of optical absorption is relatively narrow compared to the solar spectrum. Absorption coefficients are high (~105 cm -1) so that high optical densities can be achieved, at peak wavelength, with films less than 100 nm thick. Many organic materials are susceptible to degradation in the presence of oxygen or water. As one-dimensional semiconductors, their electronic and optical properties can be highly anisotropic. This is potentially useful for device design.
The first two features are due to the fact that the intermolecular van der Waals forces in organic solids are weak compared to bonds in inorganic crystals and much weaker than the intramolecular bonds. As a consequence all electronic states are localised on single molecules and do not form bands. Low mobility is aggravated by the high degree of disorder present in many organic solids. The optical excitations accessible to visible photons are usually Jr to Jr* transitions. Most conjugated solids absorb in the blue or green; absorption in the red or infrared is harder to achieve. However, the absorption bandwidth depends on the degree of conjugation and wider spectral sensitivity can be achieved in highly conjugated dye molecules. These properties impose some constraints on organic photovoltaic devices: 9 9 9 9 9
A strong driving force should be present to break up the photogenerated excitons. Low charge carrier mobilities limit the useful thickness of devices. Limited light absorption across the solar spectrum limits the photocurrent. Very thin devices mean interference effects can be important. Photocurrent may be sensitive to temperature through hopping transport and thermal dissociation of excitons.
3 Principles of Operation and Device Concepts 3.1
The simplest device structure is a layer of organic material sandwiched between two different conducting contacts, typically indium tin oxide (ITO) and a low work function metal such as A1, Ca or Mg (Figure 1). The difference in work function provides an electric field which drives separated charge carriers towards the respective contacts (in rough analogy to a p - i - n junction in
Solar Cells: Materials, Manufacture and Operation
Figure 1 Schematic energy-band diagram of a simple device consisting of a single organic layer between two metal contacts. An electricfield results from the difference in work functions of the contacts. Absorbed photons generate excitons which diffuse towards one or other contact where they may dissociate to yield charge pairs. Only the layer of organic material which lies within an exciton diffusion length of a contact can contribute to the photocurrent.
amorphous silicon). This electric field is seldom sufficient to break up the photogenerated exciton. Instead the exciton diffuses within the organic layer until it reaches a contact, where it may be broken up to supply separate charges, or recombine. Since exciton diffusion lengths are short, typically 1-10 nm, exciton diffusion limits charge carrier generation in such a device. Photocarrier generation is therefore a function not only of bulk optical absorption, but also of available mechanisms for exciton dissociation. Other loss factors are nonradiative recombination at the interfaces and non-geminate recombination at impurities or trapped charges. Single layer solar cells of this type typically deliver quantum efficiencies (QE) of less than 1% and power conversion efficiencies of less than 0.1%. (QE is the ratio of electrons delivered to the external circuit per incident photon of a given wavelength, and is the figure of merit in organic photovoltaics. High QE is a necessary, though not sufficient, condition for high photovoltaic efficiency. In
IIe-2- Organic and Plastic Solar Ceils
organic devices the value is still far from the values of 80-90% typical in inorganic solar cells.) 3.2
Most of the developments that have improved performance of organic photovoltaic devices are based on donor-acceptor heterojunctions. At the interface between two different materials, electrostatic forces result from the differences in electron affinity and ionisation potential. If both electron affinity and ionisation potential are greater in one material (the electron acceptor) than the other (the electron donor) then the interracial electric field drives charge separation (Figure 2). These local electric fields are strong and may break up photogenerated excitons provided that the differences in potential energy are larger than the exciton binding energy. In a planar heterojunction, or 'bi-layer' device, the organic donor-acceptor interface separates excitons much more efficiently than the organic-metal interfaces in a single layer device and with very high purity materials, photovoltaic devices with high QE may be made. 3.3
A revolutionary development in organic photovoltaics (and photodetectors) came in the mid 1990s with the introduction of a dispersed hetero)unction, where an electron accepting and an electron donating material are blended
Figure 2 Schematic energy-band diagram of a donor-acceptor heterojunction. If both the excited state (LUMO) and ground state (HOMO) of the donor material lie at energies sufficiently higher than those of the acceptor material, then it is energetically favourable for an exciton reaching the interface to dissociate, leaving a positive polaron on the acceptor and a negative polaron on the donor. For efficient photocurrent generation, charge separation (2) should compete successfully with geminate recombination (4) after a photon absorption event ( 1 ), and transfer to contacts (3) should compete with interracial recombination (5).
Solar Cells: Materials, Manufacture and Operation
together. If the domain size in either material is similar to the exciton diffusion length, then wherever an exciton is photogenerated in that material, it is likely to diffuse to an interface and break up. If continuous paths exist in each material from the interface to the respective electrodes, then the separated charge carriers may travel to the contacts and deliver current to the external circuit (Figure 3(a)). This effect was reported independently by several groups [5-7] for a blend of two conjugated polymers. The blend improved QE to around 6-8% from less than 1% for either polymer alone. Around the same time, Yu and co-workers reported a QE of 29% for a blend of the hole transporter, poly-phenylene vinylene (PPV), with a derivative of C6o , where the C6o acts as the electron transporting component (Figure 3 (b)). This was followed by observations of enhanced QE in heterojunctions made from conjugated polymers with inorganic nanocrystals [9,10] and organic dye crystals . The demonstration of improved QE with dispersed heterojunctions represents a departure from the device physics of conventional solar cells and has led to new device and materials designs. The principles of operation are shared by dye sensitised solar cells which are discussed in reference [ 12 ] and Chapter IIe- 1.
4 Leading Device Designs The early 2000s have seen developments in the synthesis of new photovoltaic materials; the combination of materials into new device architectures; studies of the effect of processing conditions and other factors on morphology and performance; and manipulation of materials at a molecular level, exploiting molecular self assembly and modification of interfaces. During this period power conversion efficiencies of over 3% have been reported in four distinct classes of device and QEs of over 20% achieved in several others. Several studies of issues relating to production, field performance and stability have been reported. Progress has been made with the understanding of photocurrent generation and charge separation, and the first approaches to developing a device physics for organic solar cells, have been made. At time of writing, organic solar cell technology is young and the field is still wide open. Several very different device designs are competing as front runners and it is too early to guess which, if any, of these will emerge as a serious contender for commercialisation. Below we summarise the main features of the most promising options. Power conversion efficiencies of over 3% have now been achieved in the three classes of device listed below and in Table 1. (High power conversion efficiencies have been reported [13,14] for a fourth class, a Schottky barrier device made from a doped molecular crystal in contact with an n-type a metal or n-type oxide layer, but these results are still unconfirmed.) (1) Planar heterojunction devices made by vacuum deposition of thin films of small molecules have been studied by several groups, for application to LEDs as well as solar cells. An impressive result has been achieved at Princeton with a
Organic and Plastic Solar Cells
AI . . . . . . . . . .
Electric field Figure 3 Donor and acceptor materials may be blended together to yield a dispersed heterojunction. If the domain size in the blend is similar to the exciton diffusion length, then the probability that an exciton will reach the interface and dissociate is high. For efficient photocurrent collection, each material must provide a continuous path for the transport of separated charge to the contacts. Isolated domains can trap charges, causing recombination. (a) A blend of two polymers. (b) A blend of one polymer with electron accepting nanoparticles orfullerenes. The concentration of nanoparticles should be sufficient to allow percolation.
four layer heterojunction, containing wide band gap hole transporting and electron transporting 'window' layers [15, 16]. These buffer layers function to block excitons from lossy metal contacts and to enhance optical field strength in photoactive layers via interference effects. Subsequent research on the same
Solar Cells: Materials, Manufacture and Operation
materials system has shown that greatly increased voltages can be achieved using tandem structures with tunnel junctions made from nanoparticulate silver. [ 17]. (2) Blends of polyphenylenevinylene derivatives and methanofullerenes are a well studied combination and are under intense development at Linz . Photon absorption in the polymer is followed by electron transfer to the fullerene on a sub ps time scale. Current collection depends on charge percolation through the fullerene network and the polymer matrix and is therefore critically dependent upon the blend ratio and the degree of phase separation. The combination of poly(2-methoxy-5-(3', 7'-dimethyloctyloxy)-l-4-phenylene vinylene), (MDMOPPV) with 1-(3-methoxycarbonyl)-propyl- 1-phenyl-(6,6)C61 (PCBM) appears to be a promising materials system. A breakthrough was achieved in 2 O01 by using chlorobenzene as a solvent in place of toluene, leading to QE of over 50% and power conversion efficiency of 2.5% . The much improved performance is attributed to improved phase separation with chlorobenzene. Further development led to increased open circuit voltages by using LiF interfacial layers, leading to power conversion efficiencies exceeding 3% at 50~ . (3) Solid-state dye-sensitised solar cells (DSSC) are the most promising amongst organic-inorganic composite devices to date. In the DSSC three active materials are used: an organic dye as light absorber, a nanocrystalline metal oxide film as electron transporter and liquid or organic hole transporting material (HTM) [ 12 ]. The original design used a redox active liquid electrolyte for hole transport, but a non volatile HTM is desirable for commercialisation. The ideal material should regenerate the photo-oxidised dye quickly and transport holes with high mobility. Candidates for solid state HTMs include doped arylamine based small molecules (OMeTAD)  and polythiophenes . A power conversion efficiency of 2.5% using OMeTAD was reported by the EPFL group in 2001 , greatly improving on earlier studies of that material. The improvement is attributed to the suppression of electron-hole recombination at the metal oxide surface using adsorbed pyridine. The efficiency of this system was raised to over 3% by using silver ions to increase the density of adsorbed dye molecules on the TiO2 surface, so increasing both ]sc and Voc through increased photocurrent generation [23 ]. A number of other device types have achieved QE comparable with the devices in Table 1, though lower power conversion efficiencies. These include donor-acceptor polymer blend devices with well controlled morphology [24, 25], three layer donor-sensitiser-acceptor structures , inorganic-organic heterojunctions [2 7]; and liquid crystal-crystalline dye devices , all discussed below.
5 Challenges in Materials and Device Design Table 1 shows that whilst organic solar cells produce quite respectable opencircuit voltages, the short circuit photocurrent and fill factor are much lower than those available from inorganic devices. The lower photocurrent is due to poorer light absorption as well as photocurrent generation and transport;
~ 4.a C~
He-2 - Organic and Plastic Solar Cells
SolarCells: Materials, Manufacture and Operation
the fill factor is due to poor transport and recombination. Most current research on organic photovoltaic materials and devices is therefore focussed on the following goals: 9 9 9 9
Improving light harvesting. Improving photocurrent generation. Improving charge transport. Understanding device function and limits to performance.
Approaches to processing technology and stability are discussed in Sections 7 and 8.
5.1 Light Harvesting A preferred strategy is to replace conducting polymers in devices with others which absorb further into the red. In the polymer-fullerene cell, lower optical gap replacements for the PPV derivatives, include polythiophene derivatives , polypyrrole/thiazadole copolymers  and thiophene/naphthene copolymers [31 ]. (Polythiophenes are of general interest as the hole transporting component in a blend, on account of both their red absorption and good hole mobilities when aligned.) Special red absorbing polymers may be developed for photovoltaic applications, including copolymers with mixed properties, such as a hole transporting backbone with red absorbing side groups. Another approach is to replace the electron transporting polymer in a blend with conjugated crystalline dyes, such as anthracene or perylene, with wider absorption bands . Extended red absorption can also be achieved using red absorbing inorganic semiconductor nanoparticles. Cadmium selenide nano-rods extend absorption to 700 nm . Copper indium diselenide is particularly attractive on account of its very low band gap (~1 eV in the bulk) and is now being used in polymer-nanoparticle blends . Dye sensitisation is a different strategy where a monolayer of a third material, usually an organic dye, is introduced between donor and acceptor to function as light absorber. Since light absorption and charge transport are carried out by different materials, the light absorber does not need to be a good bulk transporter of charge. Efforts to improve light harvesting in DSSCs include development of alternative dyes and combinations of dyes. A similar concept, of an all-organic donor-absorber-acceptor structure was proposed by Yoshino . A different approach is to maximise the absorption of incident photons in the organic layers. From the perspective of light absorption, organic photovoltaic films are different from inorganic structures in the following important respects: 9 9
Films are sufficiently thin that interference occurs within the layered device, allowing for the design of light trapping structures. Films are optically anisotropic.
IIe-2- Organic and Plastic Solar Cells
Light trapping structures improve the capture of photons in the active layers through constructive interference. They allow thinner photovoltaic films to be used, and this improves the efficiency of charge transport and collection. The possibilities for light trapping for organic solar cells are discussed by Inganas . Some of these have been investigated using embossed polymer layers for light trapping [36, 37] and exploiting interference effects inside cavities made from photoactive and optically transmitting organic layers [15, 38]. Embossed polymer light trapping structures are already used in thin film silicon solar cells. Optical anisotropy is important for illumination at large angles, and is relevant to the use of plastic solar cells in diffuse light conditions. In the case of spin cast polymers, the conjugated backbone is likely to be lying in the plane of the film  with the result that light incident at large angles is less likely to be absorbed than in an isotropic material. For columnar structures such as discotic liquid crystals, anisotropy enhances absorption of light incident at wide angles. Both effects need to be considered when designing organic photovoltaic devices. Calculation of optical absorption is non-trivial, and relies on good data for the optical functions of the films, usually provided by optical ellipsometry. Figure 4 shows how absorption of light in a thin organic film can be affected by interference.
5.2 Improving Charge Transport Charge transport is limited by the low intrinsic mobilities of organic solids, and by the charge trapping effects of impurities and defects. In several recent studies, higher mobility polymers such as fluorene-triarylamine and thiophene copolymers have been used to replace MEH-PPV in blend devices [40, 41]. Materials with ordered phases offer high, though anisotropic, mobilities and in this respect liquid crystals [28, 42] and polymers with liquid crystal phases, such as polythiophenes [43 ], are interesting. Because organic electron mobilities are generally very poor, an inorganic electron transporting component may be preferred. Thin film [27, 44, 45] and dispersed nanocrystalline  Ti02 has been used in several approaches. Ti02 is particularly interesting as a cheap and non-toxic material which is stable in oxygen, can be prepared as rigid nanostructured templates, can be used in light trapping structures, and benefits from a wide experience base due to dye sensitised solar cell research. Efficient charge transfer to Ti02 from various polymers has been reported (MEH-PPV [10, 46], phenyl-amino-PPV , polythiophene ) and the sensitisation of other oxides such as Sn02 with polymers has been demonstrated [4 7]. Elongated crystalline components are attractive as electron transporters if crystal size and orientation can be controlled. Blend devices using needle-like crystalline dyes [32, 48], CdSe nano-rods  and carbon nanotubes [49, 50] have been studied. Meanwhile, organic electron transporters with improved mobility and stability are being developed.
430 Solar Cells: Materials, Manufacture and Operation
Figure 4 Interference effects influence light harvesting in layered structures. Shown is the fraction of 500 nm light absorbed in a layer of MEH-PPV of thickness d, sandwiched between glass and aluminium contacts. Interference effects are clear in the shape of the attenuation curve for films of less than 200 nm thick. Notice that afilm of 5Onto is able to absorb 55% of the light, whilst if interference were neglected 200 nm of material would be needed to absorb the same fraction of the light.
5.3 Control of
In a dispersed heterojunction device, both photocurrent generation and charge transport are functions of morphology. Photocurrent generation requires blending on the scale of the exciton diffusion length while transport requires continuous paths from interface to contacts. In polymer-nanocrystal or polymer-fullerene blends, the concentration of the particulate component should be sufficient for charge percolation [9, 51]. One attractive hypothetical configuration is a set of interdigitated electron and hole transporting channels, directed perpendicular to the contacts (this is one motivation for the study of rod-like nanocrystals). Another is a compositionally graded blend with an excess of donor type material on one side and acceptor type on the other. This concept has been demonstrated by Yoshino using vacuum deposited layers , and by Granstrom for a laminated assembly . The concept was taken further by Takahashi and co-workers who reported OE of 49% for a three layer structure where electron and hole transporting layers are separated by a heterodimer light absorbing layer . The absorbing layer is polarised upon light absorption to drive the charges towards the appropriate transport layers. This is essentially an all-organic version of the dye-sensitised solar cell. Some different morphologies are illustrated in Figure 5. In practice many materials tend to segregate when blended, and much attention has focussed on ways of controlling the morphology of blends. Routes include:
IIe-2 - Organic and Plastic Solar Ceils
Figure 5 Some approaches to improved charge separation and collection in organic solar cells. In each figure the direction of photocurrent generation is from top to bottom and the electron accepting component is shaded. (a) A compositionally graded blend improves the collection of positive and negative charges near the respective contacts [6, 24]. (b) Elongated electron acceptors such as nano-rods or dye crystals can improve electron transport [32, 33], but for efficient collection they should be directed perpendicular to the contacts. (c) Selforganising discotic liquid crystals are one way of achieving preferential charge transport perpendicular to the contacts . (d) A light absorbing dimer designed to drive positive and negative charges apart after photoexcitation can help to channel respective charges towards electron transporting and hole transporting layers .
Control of blend morphology through processing conditions. Choice of solvent, atmosphere and substrate temperature strongly influence the morphology of polymer blends [40, 41]. Choice of solvent appears to influence segregation of fullerenes in MDMO-PPV [ 18 ]. Self organisation. Self assembly by discotic liquid crystals , and by ionically or electrostatically interacting monolayers [52, 53] have been used to construct structured heterojunctions. Self-assembled monolayers can also be used to modify substrate surfaces to control the segregation of blend components . Synthesis of donor (D)-acceptor (A) copolymers (such as polymer with pendant fullerene groups ) and block copolymers. Positioning D and A groups on the same polymer backbone can ensure effective photoinduced D ~ A electron transfer under all conditions and avoids the problems of phase segregation. D-A copolymers may be designed to absorb longer wavelength photons than single polymers, so improving light harvesting, but charge extraction may be more difficult.
SolarCells: Materials, Manufacture and Operation
Use of porous organic or inorganic films as templates (for example, ). Cosublimation of small molecules to form graded D-A heterostructures [56,57]. Novel characterisation techniques have been developed to study blend morphology, including spatially resolved fluorescence  and confocal Raman spectroscopy [ 58] as well as AFM and SEM imaging techniques. 5.4 Understanding Function
Understanding of the device physics of organic solar cells is still at a primitive stage, compared to inorganic solar cells. As a basis for device physics, consider the steady-state continuity equation which describes the charge carrier population in any photonic device: 1 q
-V.] v + G- U = 0
where p is the density of carriers of charge q, Jp the current density, G the volume generation rate and U the recombination rate. For crystalline inorganic p-n junction devices, G can be equated with the local photon absorption rate, and minority carrier recombination and current terms are linear in the carrier density. In organic devices, the description of all three terms is more complicated. Charge carrier generation, G, can be related to exciton generation if the exciton lifetimes and diffusion lengths, and exciton dissociation efficiencies at interfaces, are known. In planar structures, charge carriers are effectively generated only at the interface (Figure 6) and photocurrent generation can be interpreted in terms of a filter effect . This effect may cause higher photocurrents to result from thinner films, in contradiction to the usual case. In blends, photocurrent generation is a function of interface morphology. In the ideal blend, all photogenerated excitons are dissociated by nearby interfaces, and charge carrier generation is equivalent to light absorption. (Ultrafast transient spectroscopy has been used to demonstrate the fast (sub ps) rate and high yield of charge separation in well dispersed blends, such as polymer-fullerene structures .) In all cases interference should be accounted for in calculating the exciton generation profile. Because organic materials are seldom heavily doped, charge recombination, U, is a bimolecular process. However the kinetics may be influenced by the trapping of charge at defects in the disordered material or competing recombination and transport pathways, and need to be measured for each new material system. Transient optical spectroscopy has proved useful for monitoring the rate of charge recombination in dye sensitised devices  and polymerfullerene structures , as has electron spin resonance . In the case of MDMO-PPV/PCBM structures under solar illumination, recombination appears
IIe-2 - Organic and Plastic Solar CeUs 433
Figure 6 Schematic exciton generation, charge generation and current density profiles for bi,layer structure. Exciton generation follows the absorption of light in the two materials (dashed line). Charge carrier generation occurs only at the interface, leading to delta function profiles for negative charge generation in the acceptor material (black line) and positive charge generation in the donor material (grey line). These narrow charge generation region lead to constant, unipolar currents in the respective materials, and a bimolecular recombination zone located at the interface. The amplitude of the charge generation and therefore the current depends upon the exciton diffusion length and thickness of the front (acceptor) layer. For short exciton diffusion lengths, thinner layers result in higher photocurrents.
to be dominated by the release of positive polarons from trap states and U is a superlinear function of the polaron density. The current term, 1, depends upon the relative contributions of drift and diffusive currents and charge trapping, as well as upon the morphology of donor-acceptor heterostructures. Many organic conductors exhibit dispersive charge transport characteristics, so that both diffusive and drift currents are non-linear functions of carrier density. In blends, charge carrier mobilities are also dependent upon blend composition [6 3 ]. The relative importance of drift
Solar Cells: Materials, Manufacture and Operation
and diffusive currents at photovoltaic operating conditions is not well known, but recent work [64, 65] indicates that in planar heterojunctions the driving force due to charge carrier generation at the interface may dominate over the electrostatic driving force due to difference in work function of the contacts, and may dominate the open circuit voltage (Figure 6). This is in contrast with single layer devices where photovoltage is limited by the difference in work functions of the electrode materials, but in agreement with experimental studies of polymerfullerene blends which show that the photovoltage depends upon the electron affinity of the acceptor rather than the work function of the cathode . This indicates that photocurrent collection in donor-acceptor blends does not require a macroscopic electric field, a situation which is largely agreed to apply to dye sensitised solar cells . Charge trapping further influences current through its influence on the electric field distribution. On the whole, the device physics of organic solar cells is complicated by uncertainties in material parameters, the effects of heterojunctions and interfaces on materials, and the effects of light, bias and ageing. Further understanding and the development of appropriate models will require further fundamental experimental studies on model systems.
6 Organic Photovoitaic Modules Plastic solar cells are first likely to be commercialised for low-power, consumer applications, which currently take up about 10% of the market. In this they will compete (most directly) with amorphous silicon (a-Si), and to a lesser extent with emerging thin film technologies. Plastic solar cells may offer advantages over a-Si, in lower production cost, in ease of deposition onto flexible substrates or as conformal coatings on to building materials, or in colour, and these may open up new areas in the consumer photovoltaics market. Examples of applications might be power supplies for displays and monitors, control electronics, mobile communications, battery chargers, thermoelectric coolers, various consumer products, and photovoltaic windows and other architectural materials. The modules could be integrated into appliances or building materials. In such applications the module would be designed for the specific power output required and would consist of a small number of cells in series, depending on the operating voltage required. Note that since organic solar cells deliver relatively high voltages, any given operating voltage may be achieved with fewer cells than for inorganic materials. Whether cells need to be connected in parallel depends upon the current output required. The high series resistance of ITO coated flexible substrates ( 1 0 - 1 0 0 f2 cm 2) place a limit on the useful cell area before unacceptable power loss to series resistance. With a short circuit current density of 10 mA cm -2 at one sun (a reasonable goal for organic photovoltaics), this limit might be a few tens of cm 2. However, initial applications for plastic solar cells are likely to be designed for low light levels, such as indoors. The lower illumination levels (indoor illumination is typically less than one tenth of AM1.5 intensity) lead to lower current densities and lower
IIe-2 - Organic and Plastic Solar Cells
series resistance penalties, and may avoid the need for parallel connections for current ratings of less than, say, 1 O0 mA. Modules would be produced directly during cell production (discussed below) whether a batch or a continuous process. Cell interconnects can be integrated into the modules by etching the conductive substrate, scribing the photoactive layers and pattering the top contacts during production, much as is done for inorganic thin films. After metallisation the cell material must be encapsulated in a barrier coating to protect against moisture and oxygen, and in an outer coating appropriate to the intended environment. Outer plastic encapsulants may be used as passive optical concentrators to enhance the amount of light absorbed in the thin active layers the cell. In the case of building integrated modules such as windows or roofing tiles, the deposition of contacts, photoactive layers and cell interconnections could be integrated into the production process for that component. Again, cell sizing and connections will be a function of the expected current output and power requirements. Although there is as yet no commercial production of organic solar cells, prototype plastic solar modules have been produced at the University of Linz, consisting of several cells in series, with a cell area of a few tens of cm 2. Studies of the effects of increasing cell area  show that polymer-fullerene cells can be scaled up to 150cm 2 without large losses in performance. Production of standard 12 or 24 V dc modules for power generation using plastic photovoltaic materials is still remote. The low efficiency of organic solar cells leads to larger area requirements for power generation, and higher relative costs for the balance of system components. The lower lifetime expectations also increase the cost per kWh. For these reasons organic solar cells are not foreseen to be competitive with inorganic materials for high power applications at least until the obstacles to efficiency and lifetime are overcome.
7 Production Issues The main driver for organic solar cell development has been the prospect of fabricating large area devices at low cost using production techniques developed for conventional plastics. However, there is as yet no experience in large scale organic cell production, and the following discussion is largely speculative. We discuss below established organic device production technologies which could be applied to photovoltaics, several other approaches which have been explored only in the laboratory, and hypothetical production schemes which are so far untested. 7.1 General Issues
Issues for organic solar cell production are: Conductivity, transmissivity and impermeability to oxygen and water are required. The most widely used material is ITO coated poly(ethylene terephthalate) (PET) which is already used as a
SolarCeils: Materials, Manufacture and Operation
substrate for flexible amorphous silicon solar cells. ITO is limited by a transmissivity of around 80-90% in the visible and a relatively high resistivity (typically 10-50 fl cm 2) which leads to series resistance limitations, as mentioned above. Film forming properties and electrical contact are improved by coating the ITO with a layer of the doped conducting polymer PEDOT:PSS, though this introduces an additional processing stage. New organic transparent conducting coatings are being studied, but do not yet compete with ITO. Ease of deposition. In principle, deposition of films from solution is easier and cheaper than that from the gas phase, therefore solution processible materials are preferred. 'One pot, one shot' approaches to deposition of donor-acceptor blend films, where both components are deposited from a single solution, are attractive and enable much easier processing than the sequential deposition of separate layers. In such approaches the use of self assembling materials such as discotic liquid crystals  or solvent controlled blend segregation (e.g. ) can help control the resulting blend morphology. Chemical stability. Many conjugated organic solids are unstable in the presence of oxygen and light, and may also be sensitive to water. Devices for research are preferentially fabricated in an inert and dry atmosphere, but maintaining such conditions for large-scale production is costly. Costs could be reduced by finding materials which are sufficiently stable so that devices can be prepared in ambient conditions before encapsulation. Encapsulation. Coatings are needed which are sufficiently impermeable to moisture and oxygen. This is a problem with organic substrates such as PET which are intrinsically permeable. Recent progress in development of barrier coatings for flexible OLEDs, usually using multiple deposition of organic and inorganic layers to achieve the required combination of flexibility and impermeability , has enabled plastic OLED lifetimes approaching 4000 hours . Such coatings may be used for plastic photovoltaic devices. Processing temperature. High temperature processing stages are costly and damaging to organic films. This may be an issue for solid state dye sensitised solar cells, where electrical contact must be achieved within the metal oxide film without the usual high temperature sintering stage.
The production technology depends upon the materials system used. For dry deposition of photoactive layers, a batch process similar to that used for organic light emitting diodes (OLEDs) could be used. For deposition from solution, batch or continuous processes are in principle possible, although there is as yet no industrial experience in this. 7.2 Production Processes for Molecular Films
Batch or semi-batch processes are already routinely employed for production of OLEDs. The organic materials used are layers of 'small molecules' which can be
IIe-2 - Organic and Plastic Solar Cells
evaporated on to the conducting glass substrate, followed by top metal electrodes. The devices are encapsulated in a stainless steel can using an epoxy resin before separation into individual devices. In this process the most expensive stage is the v a c u u m evaporation, since m a n y expensive v a c u u m c o m p o n e n t s are required in order to m a i n t a i n high v a c u u m ( ~ 1 0 -6 torr). Batches of area ~ 3 7 0 x 4 7 0 m m 2 are processed this way. Solar cells or modules could be produced by the same techniques. The process for solar cells should be m u c h simpler since (a) the device unit area (pixel) is m u c h larger and the fine interconnections needed to address OLEDs are not needed, and (b) the n u m b e r of molecular layers needed is lower (for a colour OLED, more t h a n three electroactive materials are needed as well as contact layers). Nevertheless the process would still be expensive for solar cell production, on a c c o u n t of the high capital and m a i n t e n a n c e costs of the v a c u u m chamber. A typical batch process for deposition on glass is s u m m a r i s e d below in Table 2. The procedures on plastic substrates would be different, and include additional e n c a p s u l a t i o n stages. An alternative to v a c u u m deposition for small molecules is organic vapourphase deposition (OVPD). Molecules are carried in a flowing gas at high temperature (~300~ and condense on to a cool substrate. Compared to v a c u u m deposition, the technique does not require high v a c u u m nor high m a i n t e n a n c e costs, it can enable large area coating and it m a y be compatible with c o n t i n u o u s processing. Films of a few tens to h u n d r e d s of n m can be produced and surface r o u g h n e s s can be minimised by controlling the flow rate. The applicability of the technique to multilayer OLED fabrication has been d e m o n s t r a t e d [ 71 ].
7.3 Batch Production Processes for Polymer Films W h e n the active materials are available in solution, n e w deposition techniques are available w h i c h m a y greatly reduce costs. Deposition from solution is more viable for solar cells t h a n for LEDs because of the larger device unit area and facile interconnections.
in a typical
Pre process Post process Encapsulation process Module process
- Clean substrate - Etching of bottom contact patterns - Building ofpassivation layer and cathode separator by photolithography - Evaporation of molecular layers -Evaporation of top contacts - Attachment of desiccant film - Alignment of stainless steel casing. - Bonding of can to substrate. - Scribing into individual devices -Connection to flexible printed circuit board - Reliability test
Solar Cells: Materials, Manufacture and Operation
For research devices, spin coating is commonly used, but this is uneconomical for large areas because of the material waste. Some of the following production techniques have been considered: 9
Doctor blading or 'wire' blading. A rod is drawn over a line of the polymer solution, to spread it out into a thin sheet. This process works well for films of 1 /zm thickness, but for thicknesses of a few 100 nm, uniform thicknesses are harder to achieve. Thinner films may be achieved using a rod loosely wrapped with wire of a given thickness. The wire supports the rod and determines the thickness of the resulting polymer film. These approaches are being investigated at Linz. Screen printing. A fine mesh screen loaded with polymer solution is brought into temporary contact with the substrate and polymer solution flows across. This technique has been applied to (small area) organic solar cells made from polymer-fullerene blends, producing thin and uniform films (active layer thickness of 40 nm with a roughness of about 2 nm) . The screen printing technique is readily applied to large areas and is widely used in conventional photovo|taic cell production for contact printing. It is also being studied for depositing the metal oxide paste in dye-sensitised solar cells. However, for large area thin films, the mesh is likely to introduce thickness variations. Inkjet printing. A fine jet of polymer solution is sprayed on to the substrate in a required pattern. The technique has huge potential for organic electronic devices where fine circuit structures are required, and has been used successfully for organic thin-film transistors [ 73]. It offers precise contact definition and an easy way to deposit multiple layers. The technique could be applied to organic photovoltaic devices, although processes to achieve uniform film thickness over large areas will need to be developed (the polymer solution needs to wet the substrate surface rather than bead up). A simpler approach is printing polymer and contact materials using an embossed stamp [ 74]. This may be compatible with reel-to-reel processing.
Some of these techniques are illustrated in Figure 7. 7.4 Continuous Production Processes for Polymer Films
Since the device structure and contact designs for organic solar cells and modules are relatively simple, the modules could be produced from solution by a continuous reel-to-reel process similar to the processes currently used to produce plastic sheeting. Such a process is particularly appropriate for solar cell applications (compared to LEDs) because large areas are required yet the contact patterns and device structures are simple. In principle, well understood production technologies can be adapted and existing plant may be redeployed to the new purpose as a way of reducing production costs. However, reel-to-reel processing has not yet been attempted for any application of organic electronic materials and experience is extremely limited.
IIe-2 - Organic and Plastic Solar Cells
Figure 7 Several possible techniques for deposition of organic photovoltaicJilms. (a) Molecular deposition in high vacuum. (b) Organic vapour phase deposition. Molecules carried in a heated gas are condensed on to cooled substrates. (c) Printing. Patterned stamps can be used to print polymerJilms of defined area. (d) Inkjet printing. This allows veryJine contact definition. (e) Doctor blading. (f) Compression between rollers.
The stages involved could be as follows (see also Figure 8): 9 9 9 9 9 9
patterned conducting coating on flexible substrate, scribe the conducting coating, deposit active layers of 1 0 0 - 2 0 0 nm thickness, scribe the active layers, deposit metal contacts by in-line sputtering at low pressure, low-temperature annealing, add the encapsulating layer by reel-to reel contact, dry and cut.
The key stage in such a process is the deposition of the active layers. The material could be deposited as a blend from a single dispenser, or from a second roller. Dispersed donor acceptor blends can be deposited from a single solution, or laminated donor-acceptor 'bi-layer' structures could be deposited by contact between rollers. As yet these processes are untried. Achieving uniform film thicknesses to within 10 nm over areas of hundreds of cm 2 represents a major challenge. An important consideration is the sensitivity of the materials to air and moisture whilst in solution. For sensitive materials the entire process could be carried out in a dry and inert atmosphere, but this adds to the cost of the plant. A number of other industrial techniques are relevant to the development and production of organic photovoltaics. An example is the use of combinatorial techniques to screen different materials combinations and select the best ones .
Solar Cells: Materials, Manufacture and Operation
Figure 8 A hypothetical reel-to-reel process. A thin layer of polymer solution is deposited on a conducting substrate, followed by deposition of top metal contacts by a process such as in-line sputtering. Barrier coatings can be applied by a second roller. Scribing of layers to interconnect cells into modules can be integrated into the process (not shown).
8 Stability and Performance Organic solar cells suffer from instability in two main respects. First, many conjugated materials are unstable in the presence of oxygen and light. The photogenerated exciton is capable of reducing oxygen, generating reactive products (such as superoxide) which react with the molecular material and chemically degrade it. The second is the mechanical instability of donor-acceptor blends. On casting the components are frozen into a non-equilibrium configuration. Over time, the components may segregate, reducing the degree of blending and the effectiveness of charge separation. The latter is a particular problem with polymer-fullerene blends, where the fullerenes tend to cluster. As yet there is no general solution to the problem of the photostability of conjugated solids. One option is to develop or to use more stable components. Some conjugated dye molecules, liquid crystals and inorganic nanocrystals offer better stability. Until more air stable materials can be developed, devices need to be encapsulated using barrier coatings, as discussed above. An alternative approach is to incorporate sacrificial oxygen scavenging components into the device, such as TiO2 or other metal oxides. The TiO2 in solid-state dye-sensitised cells may help to protect the organic components from degradation. Another lesson from dye sensitised solar cell research is that the photoactive components in a solar cell do not have to be extremely stable in isolation. The ruthenium based dye which is used in DSSCs is more stable in the cell configuration than in isolation [7 5]. This can be attributed to the very short lifetimes of the reactive photogenerated excited state and cation state when in the cell configuration. A similar effect is observed in polymer/fullerene blends, where the photodegradation of the polymer is slowed down by blending with fuilevenes, and again can be attributed to the removal of the reactive exciton by rapid charge separation [7 6].
IIe-2- Organic and Plastic Solar Cells 441
The most detailed stability and performance studies of organic solar cells have been carried out on polymer/fullerene systems. These indicate that under normal operation unprotected cells degrade after a few hours, encapsulated cells maintain over 50% of their initial performance for several months , degradation is accelerated by high temperatures both in the laboratory  and in the field in hot ambient conditions . However, these devices exhibit improved performance with increasing temperature, an advantage over inorganic devices which is attributed to temperature dependent mobility,  and shared by polymer blend devices [3 9] and DSSCs. Structural instability due to phase segregation in donor-acceptor blends is a function of materials, temperature and time. To some extent segregation may be minimised by choice of solvent and control of interfacial forces (as discussed in Section 5). The problem can be avoided by the use of rigidly connected porous templates such as inorganic semiconductor or metal oxide nanostructures. A common problem with new device designs of degradation of QE with increasing light intensity, so that cells perform well only under low illumination. Such behaviour is a signature of recombination mechanisms which may be due to impurities, and must be eliminated for the cells to be useful in solar conditions. Finally it is worth commenting on the measurement and characterisation of organic solar cells. On account of their poor spectral range and poor performance under high light intensities, organic photovoltaic device performance is often reported at a single wavelength and low light intensity. For new materials combinations, the figure of merit is often the QE at peak wavelength rather than the power conversion efficiency. Since wavelength and light intensity vary between reported measurements, as well as ambient conditions (vacuum or air), the comparison of device performance is difficult. Since organic solar cells are likely to be used in quite different contexts to conventional photovoltaics, for instance, under low or diffuse light levels, or in windows where partial transparency is required, the standard test condition may not be the most relevant. There is a case for establishing new measurement standards more relevant for organic solar cell measurement and calibration.
9 Conclusions Progress with organic photovoltaic materials and devices in recent years has been impressive. Power conversion efficiencies over 3% have been achieved in at least three different device structures, varying from high quality, vacuum deposited multilayer molecular films to dispersed heterojunctions in spin cast soluble polymers. All are based on the concept of a donor-acceptor system where photogenerated excitons are split by forces at the donor-acceptor interface. Higher efficiency requires improvements in absorption of red light, in charge transport and in material stability. Recent research focuses on the synthesis and testing of new photovoltaic materials in established device structures, and the development of new structures where morphology is controlled through self-assembly and processing conditions. Experience with commercial scale
SolarCeils:Materials, Manufactureand Operation
devices is still limited, as is the theoretical understanding of device function. Based on current trends, efficiencies of 5-10% appear to be within reach, although stability remains an obstacle.
Acknowledgements The author is grateful to Youngkyoo Kim, Stephen Forrest, Ralph Gottschalg and ]ames Durrant for helpful discussions, and to Felix Braun for help with Figure 4. The support of the Engineering and Physical Sciences Research Council and the Greenpeace Environmental Trust is acknowledged.
     
Heeger, A.]., 2001. Semiconducting and metallic polymers: The fourth generation of polymeric materials. 1. Physical Chemistry B, Vol. 105(36), pp. 8475-8491. Wallace, G.G. et al., 2000. Conjugated polymers: New materials for photovoltaics. ChemicaIInnovation, Vol. 30 (4), pp. 15-22. Brabec, C.J., Sariciftci, N.S. and Hummelen, J.C., 2001. Plastic solar cells. Advanced Functional Materials, Vol. 11 (1), pp. 15-26. Halls, J.J.M. and Friend, R.H., 2001. Organic Photovoltaic Devices. In: Archer, M.D. and Hill, R.D., Eds., Clean Electricity from Photovoltaics, Imperial College Press, London, pp. 3 77-445. Yu, G. and Heeger, A.J., 1995. Charge Separation and Photovoltaic Conversion in Polymer Composites with Internal Donor-Acceptor Heterojunctions. 1. Appl. Phys. Vol. 78(7), pp. 4510-4515. Yoshino, K. et al., 1997. Novel photovoltaic devices based on donoracceptor molecular and conducting polymer systems. IEEE Transactions on Electron Devices, Vol. ED-44(8), pp. 1315-1324. Halls, J.J.M. et al., 1995. Efficient Photodiodes from Interpenetrating Polymer Networks. Nature, Vol. 3 76(6540), pp. 498-500. Yu, G. et al., 1995. Polymer Photovoltaic Cells - Enhanced Efficiencies Via a Network of Internal Donor-Acceptor Heterojunctions. Science, Vol. 270(5243), pp. 1789-1791. Greenham, N.C., Peng, X.G. and Alivisatos, A.P., 1996. Charge separation and transport in conjugated polymer/semiconductornanocrystal composites studied by photoluminescence quenching and photoconductivity. PhysicalReview B, Vol. 54(24), pp. 17628-1763 7. Salafsky, J.S., 1999. Exciton dissociation, charge transport, and recombination in ultrathin, conjugated polymer-TiO2 nanocrystal intermixed composites. PhysicalReview B, Vol. 59(16), pp. 10885-10894. Petritsch, K. et al., 2000. Dye-based donor/acceptor solar cells. Solar Energy Materials and Solar Cells, Vol. 61 (1), pp. 63-72.
IIe-2 - Organicand Plastic Solar Cells 443    
 [2o1  [221
Hagfeldt, A. and Gratzel, M., 2000. Molecular photovoltaics. Accounts of Chemical Research, Vol. 33 (5), pp. 269-2 77. Schon, J.H. et al., 2000. Efficient organic photovoltaic diodes based on doped pentacene. Nature, Vol. 403(6768), pp. 408-410. Schon, J.H., Kloc, C. and Batlogg, B., 2001. Pentacene based photovoltaic devices. Synthetic Metals, Vol. 124(1), pp. 95-9 7. Peumans, P., Bulovic, V. and Forrest, S.R., 2000. Efficient photon harvesting at high optical intensities in ultrathin organic doubleheterostructure photovoltaic diodes. Applied Physics Letters, Vol. 76(19), pp. 2650-2652. Peumans, P. and Forrest, S.R., 2001. Very-high-efficiency doubleheterostructure copper phthalocyanine/C-60 photovoltaic cells. Applied Physics Letters, Vol. 79(1), pp. 126-128. Yakimov, A. and Forrest, S.R., 2002. High photovoltage multipleheterojunction organic solar cells incorporating interfacial metallic nanoclusters. Applied Physics Letters, Vol. 80(9), pp. 1667-1669. Shaheen, S.E. et al., 2001. 2.5% efficient organic plastic solar cells. Applied Physics Letters, Vol. 78(6), pp. 841-843. Brabec, C.J. et al., 2002. Effect of LiF/metal electrodes on the performance of plastic solar cells. Applied Physics Letters, Vol. 80(7), pp. 1288-1290. Bach, U. et al., 1998. Solid-state dye-sensitized mesoporous Ti02 solar cells with high photon-to-electron conversion efficiencies. Nature, Vol. 395(6702), pp. 583-585. Spiekermann, S. et al., 2001. Poly(4-undecyl-2,2'-bithiophene) as a hole conductor in solid state dye sensitized titanium dioxide solar cells. Synthetic Metals, Vol. 121 (1-3), pp. 1603-1604. Kruger, J. et al., 2001. High efficiency solid-state photovoltaic device due to inhibition of interface charge recombination. Applied Physics Letters, Vol. 79(13), pp. 2085-208 7. Kruger, J. et al., 2002. Improvement of the photovoltaic performance of solid-state dye- sensitized device by silver complexation of the sensitizer cisbis(4,4'-dicarboxy-2,2 '-bipyridine)-bis(isothiocyanato) ruthenium(II). Applied Physics Letters, Vol. 81 (2), pp. 367-369. Granstrom, M. et al., 1998. Laminated fabrication of polymeric photovoltaic diodes. Nature, Vol. 395(6699), pp. 257-260. Arias, A.C. et al., 2002. Vertically segregated polymer blend photovoltaic thin film structures through surface mediated solution processing. Applied Physics Letters, in press. Takahashi, K. et al., 2000. Three-layer organic solar cell with highpower conversion efficiency of 3.5%. Sol. Energy Mater. Sol. Cells, Vol. 61 (4), pp. 403-416. Arango, A.C. et al., 2000. Efficient titanium oxide/conjugated polymer photovoltaics for solar energy conversion. Advanced Materials, Vol. 12(22), p. 1689.
444 SolarCells:Materials, Manufactureand Operation
  
Schmidt-Mende, L. et al., 2001. Self-organized discotic liquid crystals for high-efficiency organic photovoltaics. Science, Vol. 293(5532), pp. 1119-1122. Brabec, C.J. et al., 2001. Influence of disorder on the photoinduced excitations in phenyl substituted polythiophenes. Journal of Chemical Physics, Vol. 115(15), pp. 7235-7244. Dhanabalan, A. et al., 2001. Synthesis and characterization of a low bandgap conjugated polymer for bulk heterojunction photovoltaic cells. Advanced Functional Materials, Vol. 11(4), pp. 255-262. Shaheen, S.E. et al., 2001. Low band-gap polymeric photovoltaic devices. Synthetic Metals, Vol. 121(1-3), pp. 1583-1584. Dittmer, J.J., Marseglia, E.A. and Friend, R.H., 2000. Electron trapping in dye/polymer blend photovoltaic cells. Advanced Materials, Vol. 12(17), 2000, p. 1270. Huynh, W.U., Dittmer, J.J. and Alivisatos, A.P., 2002. Hybrid nanorodpolymer solar cells. Science, Vol. 295(5564), pp. 2425-2427. Arici, E. et al., 2001. CIS Plastic Solar Cells. Proc. 17th European Photovoltaic Solar Energy Conf. Inganas, O. et al., 2001. Recent progress in thin film organic photodiodes. Synthetic Metals, Vol. 121(1-3), pp. 1525-1528. Niggemann, M. et al., 2001. Trapping Light in Organic Plastic Solar Cells with integrated Diffraction Gratings. Proc. 17th European Photovoltaic Solar Energy Conf. Roman, L.S. et al., 2000. Trapping light in polymer photodiodes with soft embossed gratings. Advanced Materials, Vol. 12 (3), p. 189. Rostalski, J. and Meissner, D., 2000. Photocurrent spectroscopy for the investigation of charge carrier generation and transport mechanisms in organic p/n junction solar cells. Sol. Energy Mater. Sol. Ceils, Vol. 63(1), pp. 37-47. Ramsdale, C.M. and Greenham, N.C., 2002. Ellipsometric determination of anisotropic optical constants in electroluminescent conjugated polymers. Advanced Materials, Vol. 14(3), p. 212. Halls, J.J.M. et al., 2000. Photodiodes based on polyfluorene composites: Influence of morphology. Advanced Materials, Vol. 12(7), p. 498. Arias, A.C. et al., 2001. Photovoltaic performance and morphology of polyfluorene blends: A combined microscopic and photovoltaic investigation. Macromolecules, Vol. 34(17), pp. 6005-6013. Struijk, C.W. et al., 2000. Liquid crystalline perylene diimides: Architecture and charge carrier mobilities. Journal of the American ChemicalSociety, Vol. 122(45), pp. 11057-11066. Videlot, C., E1Kassmi, A. and Fichou, D., 2000. Photovoltaic properties of octithiophene-based Schottky and p/n junction cells: Influence of molecular orientation. Sol. Energy Mater. Sol. Cells, Vol. 63(1), pp. 69-82. Thelakkat, M., Schmitz, C. and Schmidt, H.W., 2002. Fully vapordeposited thin-layer titanium dioxide solar cells. Advanced Materials, Vol. 14(8 ), pp. 577-581.
IIe-2- Organicand PlasticSolarCells 445  
[521    [561
Fan, Q. et al., 2001. A solid state solar cell using sol-gel processed material and a polymer. ChemicalPhysics Letters, Vol. 347(4-6), pp. 325-330. Savenije, T.J., Warman, J.M. and Goossens, A., 1998. Visible light sensitisation of titanium dioxide using a phenylene vinylene polymer. ChemicalPhysics Letters, Vol. 287(1-2), pp. 148-153. Anderson, N.A. et al., 2002. Subpicosecond photoinduced electron transfer from a conjugated polymer to SnO2 semiconductor nanocrystals. Physica E, Vol. 14, pp. 215-218. Cabanillas-Gonzales, J. et al., 2003. Effect of aggregation on photocurrent generation in polyfluorene doped with violanthrone. Synthetic Metals, Vol. 137, pp. 1471-1472. Ago, H. et al., 1999. Composites of carbon nanotubes and conjugated polymers for photovoltaic devices. Advanced Materials, Vol. 11(5), pp. 1281. Lee, S.B. et al., 2001. Electrical and optical properties of conducting polymer-C-60 carbon nanotube system. Synthetic Metals, Vol. 12(1-3), pp. 1591-1592. Brabec, C.J. et al., 1999. Photovoltaic properties of conjugated polymer/ methanofullerene composites embedded in a polystyrene matrix. ]. Appl. Phys., Vol. 85(9), pp. 6866-6872. Baur, J.W. et al., 2001. Photovoltaic interface modification via electrostatic self- assembly. Synthetic Metals, Vol. 121(1-3), pp. 1547-1548. Schroeder, R. et al., 2001. Control of excited state dynamics in ionically self-assembled monolayers of conjugated molecules. Synthetic Metals, Vol. 121(3), pp. 1521-1524. Ramos, A.M. et al., 2001. Photoinduced electron transfer and photovoltaic devices of a conjugated polymer with pendant fullerenes. ]ournal of the American Chemical Society, Vol. 123(2 7), pp. 6714-6715. de Boer, B. et al., 2001. Synthesis and self-organization of PPV-based block copolymers for photonic applications. Synthetic Metals, Vol. 121 (13), pp. 1541-1542. Murgia, M. et al., 2 O01. Intedigitated p-n junction: a route to improve the efficiency in organic photovoltaic cells. Synthetic Metals, Vol. 121 (1-3), pp. 1533-1534. Pfeiffer, M., et al., 2000. Controlled p-doping of pigment layers by cosublimation: Basic mechanisms and implications for their use in organic photovoltaic cells. Sol. Energy Mater. Sol. Cells, Vol. 63(1), pp. 83-99. Stevenson, R., et al., 2001. Raman microscopy determination of phase composition in polyfluorene composites. Applied Physics Letters, Vol. 79(14), pp. 2178-2180. Harrison, M.G., Gruner, J. and Spencer, G.C.W., 1997. Analysis of the photocurrent action spectra of MEH-PPV polymer photodiodes.Physical ReviewB, Vol. 55(12), pp. 7831-7849.
446 SolarCells:Materials,Manufactureand Operation
[6o]    
Nogueira, A.F. et al., 2001. Electron transfer dynamics in dye sensitized nanocrystalline solar cells using a polymer electrolyte. Journal of Physical Chemistry B, Vol. 105(31), pp. 7517-7524. Montanari, I. et al., 2002. Transient optical studies of charge recombination dynamics in a polymer/fullerene composite at room temperature. Applied Physics Letters, Vol. 81(16), pp. 3001-3003. Dyakonov, V. et al., 2 O01. Spectroscopy on polymer-fullerene composites and photovoltaic cells. Synthetic Metals, Vol. 121 (1-3), pp. 1529-1532. Paci0s, R. et al., 2003. Efficient polyfluorene based solar cells. Synthetic Metals, Vol. 137, pp. 1469-1470. Ramsdale, C.M. et al., 2002. The origin of the open-circuit voltage in polyfluorene-based photovoltaic devices. Journal of Applied Physics, Vol. 92(8), pp. 4266-4270. Gregg, B.A. and Hanna, M.C., 2003. Comparing organic to inorganic photovoltaic cells: Theory, experiment and simulation. Journal of Applied Physics, Vol. 93, pp. 3605-3614. Brabec, C.J. et al., 2001. Origin of the open circuit voltage of plastic solar cells. Advanced Functional Materials, Vol. 11 (5), pp. 3 74-380. Cahen, D. et al., 2000. Nature of photovoltaic action in dye-sensitized solar cells. Journal of Physical Chemistry B, Vol. 104(9 ), pp. 2053-2059. Padinger, F. et al., 2000. Fabrication of large area photovoltaic devices containing various blends of polymer and fullerene derivatives by using the doctor blade technique. Opto-Electronics Review, Vol. 8(4), pp. 280-283. Burrows, P.E. et al., 2001. Ultra barrier flexible substrates for fiat panel displays. Displays, Vol. 22(2), pp. 65-69. Weaver, M.S. et al., 2002. Organic light-emitting devices with extended operating lifetimes on plastic substrates. Applied Physics Letters, Vol. 81(16), pp. 2929-2931. Shtein, M. et al., 2001. Material transport regimes and mechanisms for growth of molecular organic thin films using low-pressure organic vapor phase deposition. ]. Appl. Phys., Vol. 89(2), pp. 1470-1476. Shaheen, S.E. et al., 2001. Fabrication of bulk heterojunction plastic solar cells by screen printing. Applied Physics Letters, Vol. 79(18), pp. 2996-2998. Sirringhaus, H. et al., 2000. High-resolution inkjet printing of allpolymer transistor circuits. Science, Vol. 290, pp. 2123-212 6. Kim, C., Shtein, M. and Forrest, S.R., 2002. Nanolithography based on patterned metal transfer and its application to organic electronic devices. Applied Physics Letters, Vol. 80(21 ), pp. 4051-4053. Nazeeruddin, M.K. et al., 1993. Conversion of Light to Electricity by Cis-X2bis(2,2'-Bipyridyl-4,4'-Dicarboxylate) Ruthenium(II) ChargeTransfer Sensitizers (X = CI-, Br-, I-, Cn-, and Scn-) on Nanocrystalline Ti02 Electrodes. Journal of the American Chemical Society, Vol. 115(14), pp. 6382-6390.
IIe-2- Organicand Plastic Solar Cells 447
Neugebauer, H. et al., 2000. Stability and photodegradation mechanisms of conjugated polymer/fullerene plastic solar cells. Sol. Energy Mater. Sol. Cells, Vol. 61 (1), pp. 35-42. Padinger, F. et al., 2001. Degradation of bulk heterojunction solar cells operated in an inert gas atmosphere: a systematic study. Synthetic Metals, Vol. 121 (1-3), pp. 1605-1606. Tuladhar, S.M. et al., 2001. Out-door photovoltaic characterization of plastic solar cells. Presented at the International Workshop on Nanostructures in Photovoltaics, Dresden, unpublished. Katz, E.A. et al., 2001. Temperature dependence for the photovoltaic device parameters of polymer-fullerene solar cells under operating conditions. J. Appl. Phys., Vol. 90(10), pp. 5343-5350.